- Recrystallization (metallurgy)
Recrystallization is a process by which deformed grains are replaced by a new set of undeformed grains that nucleate and grow until the original grains have been entirely consumed. Recrystallization is usually accompanied by a reduction in the strength and
hardnessof a material and a simultaneous increase in the ductility. Thus, the process may be introduced as a deliberate step in metals processing or may be an undesirable by product of another processing step. The most important industrial uses are the softening of metalspreviously hardened by cold work, which have lost their ductility, and the control of the grain structure in the final product.
A precise definition of recrystallization is difficult as the process is strongly related to several other processes, most notably recovery and
grain growth. In some cases it is difficult to precisely define the point at which one process begins and another starts. Doherty "et al" (1998) defined recrystallization as:
"... the formation of a new grain structure in a deformed material by the formation and migration of high angle grain boundaries driven by the stored energy of deformation. High angle boundaries are those with greater than a 10-15° misorientation"Thus the process can be differentiated from recovery (where high angle grain boundaries do not migrate) and
grain growth(where the driving force is only due to the reduction in boundary area).
Recrystallization may occur during or after deformation (during cooling or a subsequent heat treatment, for example). The former is termed "dynamic" while the latter is termed "static". In addition, recrystallization may occur in a discontinuous manner, where distinct new grains form and grow, or a continuous manner, where the microstructure gradually evolves into a recrystallised microstructure. The different mechanisms by which recrystallization and recovery occur are complex and in many cases remain controversial. The following description is primarily applicable to static continuous recrystallization, which is the most classical variety and probably the most understood. Additional mechanisms include (geometric)
dynamic recrystallizationand strain induced boundary migration.
Laws of Recrystallization
There are several, largely empirical laws of recrystallization:
* "Thermally activated". The rate of the microscopic mechanisms controlling the nucleation and growth of recrystallised grains depend on the annealing temperature.
Arrheniustype equations indicate an exponential relationship.
* "Critical temperature". Following from the previous rule it is found that recrystallization requires a minimum temperature for the necessary atomic mechanisms to occur. This "recrystallization temperature" decreases with annealing time.
* "Critical deformation". The prior deformation applied to the material must be adequate to provide nuclei and sufficient stored energy to drive their growth.
* "Deformation affects the critical temperature". Increasing the magnitude of prior deformation, or reducing the deformation temperature, will increase the stored energy and the number of potential nuclei. As a result the recrystallization temperature will decrease with increasing deformation.
* "Initial grain size affects the critical temperature". Grain boundaries are good sites for nuclei to form. Since an increase in grain size results in fewer boundaries this results in a decrease in the nucleation rate and hence an increase in the recrystallization temperature
* "Deformation affects the final grain size". Increasing the deformation, or reducing the deformation temperature, increases the rate of nucleation faster than it increases the rate of growth. As a result the final grain size is reduced by increased deformation.
During plastic deformation the work performed is the integral of the stress ? and the plastic strain increment d?. Although the majority of this work is converted to heat, some fraction (~1-5%) is retained in the material as defects - particularly dislocations. The rearrangement or elimination of these dislocations will reduce the internal energy of the system and so there is a thermodynamic driving force for such processes. At moderate to high temperatures, particularly in materials with a high stacking fault energy such as aluminium and nickel, recovery occurs readily and free dislocations will readily rearrange themselves into subgrains surrounded low-angle grain boundaries.The driving force is the difference in energy between the deformed and recrystallised state ?E which can be determined by the dislocation density or the subgrain size and boundary energy (Doherty, 2005):
where ρ is the dislocation density, G is the shear modulus, b is the
Burgers vectorof the dislocations, γ is the sub-grain boundary energy and ds is the subgrain size.
Historically it was assumed that the nucleation rate of new recrystallized grains would be determined by the thermal fluctuation model successfully used for
solidificationand precipitation phenomena. In this theory it is assumed that as a result of the natural movement of atoms(which increases with temperature) small nuclei would spontaneously arise in the matrix. The formation of these nuclei would be associated with an energy requirement due to the formation of a new interface and an energy liberation due to the formation of a new volume of lower energy material. If the nuclei were larger than some critical radius then it would be thermodynamically stable and could start to grow. The main problem with this theory is that the stored energy due to dislocations is very low (0.1-1 Jm-3) while the energy of a grain boundaryis quite high (~0.5Jm-2). Calculations based on these values found that the observed nucleation rate was greater than the calculated one by some impossibly large factor (~1050).
As a result the alternate theory proposed by Cahn in 1949 is now universally accepted. The recrystallised grains do not nucleate in the classical fashion but rather grow from pre-existing sub-grains and cells. The 'incubation time' is then a period of
recoverywhere sub-grains with low-angle boundaries (<1-2°) begin to accumulate dislocationsand become increasingly misoriented with respect to their neighbours. The increase in misorientation increases the mobility of the boundary and so the rate of growth of the sub-grain increases. If one sub-grain in a local area happens to have an advantage over its neighbours (such as locally high dislocation densities, a greater size or favourable orientation) then this sub-grain will be able to grow more rapidly than its competitors. As it grows its boundary becomes increasingly misoriented with respect to the surrounding material until it can be recognised as an entirely new strain-free grain.
Recrystallization kinetics are commonly observed to follow the profile shown. There is an initial 'nucleation period' "t0" where the nuclei form, and then begin to grow at a constant rate consuming the deformed matrix. Although the process does not strictly follow classical nucleation theory it is often found that such mathematical descriptions provide at least a close approximation. For an array of spherical grains the mean radius "R" at a time "t" is (Humphreys and Hatherly 2004):
where "t0" is the nucleation time and "G" is the growth rate dR/dt. If "N" nuclei form in the time increment "dt" and the grains are assumed to be spherical then the volume fraction will be:
This equation is valid in the early stages of recrystallization when "f<<1" and the growing grains are not impinging on each other. Once the grains come into contact the rate of growth slows and is related to the fraction of untransformed material (1-f) by the Johnson-Mehl equation:
While this equation provides a better description of the process it still assumes that the grains are spherical, the nucleation and growth rates are constant, the nuclei are randomly distributed and the nucleation time t0 is small. In practice few of these are actually valid and alternate models need to be used.
It is generally acknowledged that any useful model must not only account for the initial condition of the material but also the constantly changing relationship between the growing grains, the deformed matrix and any second phases or other microstructural factors. The situation is further complicated in dynamic systems where deformation and recrystallization occur simultaneously. As a result it has generally proven impossible to produce an accurate predictive model for industrial processes without resorting to extensive empirical testing. Since this may require the use of industrial equipment that has not actually been built there are clear difficulties with this approach.
Factors influencing the rate
annealingtemperature has a dramatic influence on the rate of recrystallization which is reflected in the above equations. However, for a given temperature there are several additional factors that will influence the rate.
The rate of recrystallization is heavily influenced by the amount of deformation and, to a lesser extent, the manner in which it is applied. Heavily deformed materials will recrystallize more rapidly than those deformed to a lesser extent. Indeed, below a certain deformation recrystallization may never occur. Deformation at higher temperatures will allow concurrent
recoveryand so such materials will recrystallize more slowly than those deformed at room temperature e.g. contrast hot and cold rolling. In certain cases deformation may be unusually homogeneous or occur only on specific crystallographic planes. The absence of orientation gradients and other heterogeneities may prevent the formation of viable nuclei. Experiments in the 1970s found that molybdenumdeformed to a true strainof 0.3, recrystallized most rapidly when tensioned and at decreasing rates for wire drawing, rolling and compression (Barto & Ebert 1971).
The orientation of a
grainand how the orientation changes during deformation influence the accumulation of stored energy and hence the rate of recrystallization. The mobility of the grain boundaries is influenced by their orientation and so some crystallographic textures will result in faster growth than others.
Solute atoms, both deliberate additions and impurities, have a profound influence on the recrystallization kinetics. Even minor concentrations may have a substantial influence e.g. 0.004% Fe increases the recrystallization temperature by around 100°C (Humphreys and Hatherly 2004). It is currently unknown whether this effect is primarily due to the retardation of nucleation or the reduction in the mobility of grain boundaries i.e. growth.
Influence of second phases
Many alloys of industrial significance have some volume fraction of second phase particles, either as a result of impurities or from deliberate alloying additions. Depending on their size and distribution such particles may act to either encourage or retard recrystallization.
Recrystallization is prevented or significantly slowed by a dispersion of small, closely spaced particles due to
Zener pinningon both low- and high-angle grain boundaries. This pressure directly opposes the driving force arising from the dislocation density and will influence both the nucleation and growth kinetics. The effect can be rationalised with respect to the "particle dispersion level" Fv/r where Fv is the volume fraction of the second phase and r is the radius. At low Fv/r the grain size is determined by the number of nuclei, and so initially may be very small. However the grains are unstable with respect to grain growthand so will grow during annealling until the particles exert sufficient pinning pressure to halt them. At moderate Fv/r the grain size is still determined by the number of nuclei but now the grains are stable with respect to normal growth (while abnormal growth is still possible). At high Fv/r the unrecrystallised deformed structure is stable and recrystallization is suppressed.
The deformation fields around large (<1μm) non-deformable particles are characterised by high dislocation densities and large orientation gradients and so are ideal sites for the development of recrystallization nuclei. This phenomenon, called particle stimulated nucleation (PSN), is notable as it provides one of the few ways to control recrystallization by controlling the particle distribution.
The size and misorientation of the deformed zone is related to the particle size and so there is a minimum particle size requried to initiate nucleation. Increasing the extent of deformation will reduce the minimum particle size leading to a PSN regime in size-deformation space.If the efficiency of PSN is 1 (i.e. each particle stimulates one nuclei) then the final grain size will be simply determined by the number of particles. Occasionally the efficiency can be greater than one if multiple nuclei form at each particle but this is uncommon. The efficiency will be less than one if the particles are close to the critical size and large fractions of small particles will actually prevent recrystallization rather than initiating it (see above).
Bimodal particle distributions
The recrystallization behaviour of materials containing a wide distribution of particle sizes can be difficult to predict. This is compounded in alloys where the particles are thermally-unstable and may grow or dissolve with time. The situation is more simple in bimodel alloys which have two distinct particle populations. An example is Al-Si alloys where it has been shown that even in the presence of very large (<5μm) particles the recrystallization behaviour is dominated by the small particles (Chan & Humphreys 1984). In such cases the resulting microstructure tends to resemble one from an alloy with only small particles.
Wikimedia Foundation. 2010.
См. также в других словарях:
Recrystallization — (see also crystallization) is a physical process that has meanings in chemistry, metallurgy and geology.ChemistryIn chemistry, recrystallization is a procedure for purifying compounds. The most typical situation is that a desired compound A is… … Wikipedia
metallurgy — metallurgic, metallurgical, adj. metallurgically, adv. metallurgist /met l err jist/ or, esp. Brit., /meuh tal euhr jist/, n. /met l err jee/ or, esp. Brit., /meuh tal euhr jee/, n. 1. the technique or science of working or heating metals so as… … Universalium
Dynamic recrystallization — (DRX) is a type of recrystallization process, found within the field of metallurgy. In dynamic recrystallization, as opposed to static recrystallization, the nucleation and growth of new grains occurs during deformation rather than afterwards as… … Wikipedia
Dynamic quartz recrystallization — Quartzite from Southern Appalachians. Thin section prepared by Michael Stevens. Quartz is the most abundant single mineral in the earth s crust (behind the feldspar group), and as such is present in a very large proportion of rocks both as… … Wikipedia
Annealing (metallurgy) — Annealing, in metallurgy and materials science, is a heat treatment wherein a material is altered, causing changes in its properties such as strength and hardness. It is a process that produces conditions by heating to above the recrystallization … Wikipedia
Continuous sub-grain rotation type dynamic recrystallization — In Metallurgy, Materials Science and Structural geology continuous sub grain rotation type dynamic recrystallization is recognized as an important mechanism for dynamic recrystallisation. It involves the rotation of initially low angle sub grain… … Wikipedia
Crystallization — Crystallizing and Crystallized redirect here. For the action adventure video game, see Crystalis. For the 2009 song by The xx, see Crystalised. For other uses, see Crystallization (disambiguation). Crystallization … Wikipedia
Single crystal — A huge KDP crystal grown from a seed crystal in a supersaturated aqueous solution at LLNL which is to be cut into slices and used on the National Ignition Facility for frequency doubling and tripling. A single crystal or monocrystalline solid is… … Wikipedia
Rolling (metalworking) — A rolling schematic In metalworki … Wikipedia
Deformation mechanism — In structural geology, metallurgy and materials science, deformation mechanisms refer to the various mechanisms at the grain scale that are responsible for accommodating large plastic strains in rocks, metals and other materials. Contents 1… … Wikipedia